Chapter 8

Phase Diagrams A in a is a region that differ in its microstructure and or composition from another region

Al2CuMg

Al H2O(, ) in H2O () ⇒ 2 phases • homogeneous in structure and atomic arrangement • have same chemical and physical properties throughout • have a definite and able to be mechanically separated from its surroundings

Chapter 8 in Smith & Hashemi Additional resources: Callister, chapter 9 and 10 Chapter 8 1 and “degrees of freedom”

A phase diagrams is a type of graph used to show the equilibrium conditions between the thermodynamically-distinct phases; or to show what phases are present in the material system at various T, p, and compositions • “equilibrium” is important: phase diagrams are determined by using slow cooling conditions ⇒ no information about kinetics Degree of freedom (or variance) F is the number of variables (T, p, and composition) that can be changed independently without changing the phases of the system

Phase diagram of CO2 Chapter 8 2 8.1 Phase Diagram of

3 phases: solid, liquid, vapour : 4.579 Torr (~603Pa), 0.0098oC

• Field – 1 phase • Line – phase coexistence, 2 phases • Triple point – 3 phases

Chapter 8 3 8.2 Gibbs

Gibbs' phase rule describes the possible # of degrees of freedom (F) in a closed system at equilibrium, in terms of the number of separate phases (P) and the number of chemical components (C) in the system (derived from thermodynamic principles by Josiah W. Gibbs in the 1870s)

F + P = C + 2 F is # of degrees of freedom or variance P is # of phases C is # of components

Component is the minimum # of species necessary to define the composition of the system

H2O C=1 (i) P=1, F=2; (ii) P=2, F=1; (iii) P=3, F=0 Chapter 8 4 8.3 How to construct phase diagrams? - Cooling curves

Cooling curves: • used to determine • record T of material vs time, as it cools from its molten state through solidification and finally to RT (at a constant !!!)

The of a pure

BC: plateaue or region of thermal arrest; in this region material is in the form of solid and liquid phases CD: solidification is completed, T drops

Chapter 8 5 Cooling curve for pure @ 1atm

As T ⇓: melted iron (liquid) ⇒ bcc Fe, δ (solid) ⇒ fcc Fe, γ (solid) ⇒ bcc Fe, α (RT)

Chapter 8 6 8.4 Binary systems (C = 2)

F + P = C + 2 = 4 ⇒ F = 4 - P

Degrees of freedom (F): At p = const (or T=const) p, T, composition p T F = 3 - P

T

0 weight % of B 100% composition 100% 100% A B 1. Two components are completely mixable in liquid and solid phase (form a solid state ), and don’t react chemically 2. Two components (A and B) can form stable compounds or alloys (for example: A, A B, A B, B) 2 3 Chapter 8 7 Binary Isomorphous System (C=2)

Isomorphous: Two elements are completely soluble in each other in solid and liquid state; substitutional solid state solution can be formed; single type of crystal str. exist Reminder: Hume-Rothery rules: (1) have similar radii; (2) both pure have same ; (3) similar electronegativity (otherwise may form a compound instead); (4) solute should have higher valence Example: Cu-Ni phase diagram (only for slow cooling conditions) line: the line connecting Ts at which liquid starts to solidify under equilibrium conditions : the temperature at which the last of the liquid phase solidifies Between liquidus and solidus: P =2

Chapter 8 8 53 wt% Ni – 47 wt% Cu at 1300oC

P = 1 F = 3 – P = 2

P = 2 ; F = 3 – P = 1 • contains both liquid and solid phases ⇒ neither of these phases can have average composition 53 wt% Ni – 47 wt% Cu

o •draw a tie line at 1300 C ⇒ from the graph: composition of liquid phase wL = o 45% and solid phase wS = 58% at 1300 C Chapter 8 9 8.5 The

The weight percentages of the phases in any 2 phase region can be calculated by using the lever rule Consider the binary equilibrium phase diagram of elements A and B that are completely soluble in each other

Co Mass fraction of B

Let x be the alloy composition of interest, its mass fraction of B (in A) is Cο Let T be the temperature of interest ⇒ at T alloy x consists of a of liquid (with C - mass fraction of B in liquid) and solid (C - mass fraction of B in solid phase) L ChapterS 8 10 Lever Rule (cont.)

Chapter 8 11 Q.: A Cu-Ni alloy contains 47 wt % Cu and 53% of Ni and is at 1300oC. Use Fig.8.5 and answer the following: A. What is the weight percent of Cu in the liquid and solid phases at this temperature? B. What weight percent of this alloy is liquid and what weight percent is solid?

Chapter 8 12 8.6 Nonequilibrium Solidification of Alloys

⇐ constructed by using very slow cooling conditions

Atomic is slow in solid state; as-cast microstructures show “core structures” caused by regions of different

As-cast 70% Cu – 30% Ni alloy showing a cored structure Chapter 8 13 Nonequilibrium Solidus

Solidification of a 70% Ni-30%Cu alloy Schematic microstructures at T2 and T4 Fig. 8.9, Smith Fig.8.10, Smith

• each core structure will have composition gradient α1-α7

• additional homogenization step is often required (

Chapter 8 14 8.7 Binary Eutectic Alloy System

• Components has limited solid in each other • Example: cooling 60%Pb – 40%Sn system Liquid ⎯eutectic⎯→⎯⎯_T a + b solid solution

This eutectic reaction is called an invariant reaction ⇒ occurs under equilibrium conditions at specific T and alloy composition F=0 at eutectic point

Chapter 8 15 Solubility Limit: Water-

• Changing T can change # of phases: path A to B.

• Changing Co can change # of phases: path B to D B(100,70) D(100,90) 1 phase 2 phases 10 0

80 L (liquid) 60 + L S (liquid solution 40 (solid i.e., syrup) sugar) 20 A(70, 20) Temperature (°C) 2 phases 0 0 20 40 60 70 80 10 0 Co=Composition (wt% sugar) Adapted from Callister Chapter 8 16 Binary Eutectic Alloy System

Figure 8.13, Smith Chapter 8 17 Q: A - (Pb – Sn) alloy contains 64 wt % proeutectic (α) and 36% eutectic α+β at 183oC – ∆T. Using Figure 8.13, calculate the average composition of this alloy.

Chapter 8 18 8.8 Binary Peritectic Alloy System

The points of the two components are quite different A liquid phase reacts with the solid phase to form a new and different solid phase Liquid + α→β

Chapter 8 19 Binary Peritectic Alloy System (cont.)

Chapter 8 20 8.9 Binary monotectic systems

Monotectic reaction: a liquid phase transforms into a solid phase and another liquid phase

L1 →α+ L2

Chapter 8 21 8.10 Invariant Reactions

To summarize: 5 invariant reactions (F = 0) 1. Eutectic Liquid →α+ β 2. Eutectoid α → β + γ 3. Peritectic Liquid + α→β 4. Peritectoid α + β→γ

5. Monotectic L1 →α+ L2

The eutectic and eutectoid reactions are similar in that they both involve the decomposition of a single phase into two solid phases. The –oid suffix indicates that a solid, rather than liquid, phase is decomposing.

Chapter 8 22 8.11 Phase Diagrams with Intermediate Phases and Compounds

Terminal phase: a solid solution of one component in another for which one boundary of the phase field is a pure component Intermediate phase: a phase whose composition range is between those of terminal phases

Chapter 8 23 Ti-Si-O system

• Experiment (700-1000oC)

Ti + SiO2 → Ti5Si3 and TiOy

• At equilibrium the system will be in

TiSix –TiOy –SiO2 three phase region (from calculations)

•Ti5Si3 – TiO – SiO2 three phase region determined experimentally and remaining tie lines can be inferred

Chapter 8 24 8.12 Ternary Phase Diagram

F + P = C + 2 For p = 1atm, T = const (isoterms)

Cr-Fe-Ni alloy stainless

Chapter 8 25 Three and four component system

AB + AC = 2A + BC

∆G = (2GA + GBC) – (GAB + GAC)

If ∆G <0, there is tie line between A and BC The remaining tie lines cannot cross A

AB + AC + AD = 3A + BCD

∆G = (3GA + GBCd) – (GAB + GAC + GAD)

AB AC • Two phase equilibrium is represented by a tie line • If ∆G <0, there is a tie line between A and BCD; • otherwise plane connects AB-AC-AD

B BC C Chapter 8 26 The Ti-Si-N-O quaternary phase diagram

• Entire phase diagram can be calculated by taking into account all possible combinations of reactions and products • 4 ternary diagrams of Ti-Si-N, Ti-N-O, Ti-Si-O and Si-N-O were evaluated • additional quaternary tie lines from

TiN to SiO2 and Si2N2O • stable metallization bilayer of TiN and

TiSi2 in contact with SiO2

A.S.Bhansali, et al., J.Appl.Phys. 68(3) (1990) 1043

Z.Chen, et al., Phys.Stat..B 241(10) (2004) 2253

Chapter 8 27